Magnetic Carbon Microspheres as a Reusable Adsorbent for Sulfonamide Removal from Water
© The Author(s). 2017
Received: 13 April 2017
Accepted: 28 August 2017
Published: 6 September 2017
Novel reusable magnetic carbon microspheres (MCMs) were prepared by hydrothermal method with glucose as carbon source and Fe3O4 nanoparticles as magnetic raw materials. And adsorption performance of MCMs for sulfonamide removal from water was investigated in detail. The results indicated that the calcination temperature and calcination time had significant effects on the surface area and its volume porous of MCMs. When MCMs were calcined in 600 °C for 1 h, the surface area and volume porous of MCMs were 1228 m2/g and 0.448 m3/g, respectively. The adsorption results showed that the adsorption data fitted well with the Langmuir isotherm model and followed pseudo-second-order kinetics. When the pH value was changed from 4.0 to 10.0, the adsorption capacity of MCMs for sulfonamide was decreased from 24.6 to 19.2 mg/g. The adsorption capacity of as-synthesized MCMs achieved 18.31 mg/g after it was reused four times, which exhibited a desirable adsorption capacity and reusability.
KeywordsMagnetic Carbon Microspheres (MCMs) Adsorption Sulfonamide Reusability
Pharmaceutical antibiotics are widely used in the world to treat diseases and improve the growth rate of animals. However, it has been found that antibiotics have serious adverse effects on the aquatic environment, which has attracted growing concern in recent years [1–3]. Among all the antibiotics, sulfonamide antibiotics are usually heavily used in clinical, animal husbandry and aquaculture. They are very stable and poorly absorbed in the digestive tract with only a small portion of sulfonamide antibiotics metabolized or absorbed. When they are discharged into the environment, sulfonamide antibiotics have been frequently detected in wastewater treatment plants, groundwater, surface water, soil, sediments, etc. [4–6]. The sulfonamide antibiotic residues can not only damage the environment but also pose a significant risk to human health. Therefore, it is necessary to investigate new technology to effectively removing these antibiotic residues from water.
Carbon materials have drawn much attention for their chemical inertness, biocompatibilities, and thermal stabilities [7–9]and have been investigated extensively in the field of separation, catalyst, and adsorption [10–12]. However, the traditional carbon materials are difficult to separate from solution when they are used as adsorbent. The conventional methods are mainly filtration and centrifugation, which are inconvenient and low efficient especially when the working condition is complicated. With the development of nanotechnology in recent years, carbon materials combined with nano-magnetic materials, namely magnetic carbon microspheres (MCMs), have been paid much more attention which can be easily separated using a magnet. These magnetic carbon composites have been used as adsorbents for pollutant removal from water, such as methyl blue  and phenol and nitrobenzene . Zhu et al. have reviewed the synthesis and application of magnetic carbon composites .
In this paper, we introduced a novel approach for synthesizing new magnetic carbon microspheres (MCMs) with high surface area by hydrothermal method, in which glucose and Fe3O4 nanoparticles were used as raw materials. And adsorption performance of MCMs for sulfonamide removal from water was evaluated in detail.
Chemicals and Materials
FeCl3·6H2O, ethanol, ethylene glycol, and sulfonamide were purchased from Sinopharm Chemical Reagent Co., Ltd. NaAc·3H2O, glucose, KCl, NaOH, and HCl were from Nanjing Chemical Reagent Co., Ltd. ZnCl2 was purchased from Xilong Chemical Co., Ltd. Distilled water was used in all the experiments.
Preparation of Fe3O4 Nanoparticles
Fe3O4 nanoparticles were prepared via the hydrothermal method as reported in . FeCl3·6H2O (1.35 g) and NaAc·3H2O (3.60 g) were dissolved in 40 mL of ethylene glycol to form a homogeneous solution and then was translated to a teflon-lined stainless autoclave (100 mL capacity), heated to 200 °C for 8 h. After it was cooled to room temperature, the resulting product was washed with deionized water and ethanol for three times, respectively.
Preparation of MCMs
0.1 g Fe3O4 nanoparticles, appropriate dosage of glucose, and 60 mL distilled water were added into a 100-mL beaker and then were stirred to make the Fe3O4 nanoparticles homodispersed. The solution was poured into a 100 mL autoclave and heated to 200 °C for 11 h. The MCMs obtained were washed twice with deionized water and ethanol.
MCMs were immersed in the 40% ZnCl2 solution [17, 18] and then were dried in a vacuum drying oven. The as-synthesized MCMs were putted in a tuber furnace and heated under nitrogen atmosphere. Thus, the calcinated and activated MCMs were obtained. The resulting MCMs were washed, used 50 mL deionized water five to eight times till the concentration of Zn2+ was less than 0.05 mg/L, and the MCMs were dried in a vacuum drying oven for sulfonamide adsorption.
MCMs were characterized using transmission electron microscopy (TEM, Model Tecnai 12, Philips Co., Ltd., Holland) and field emission scanning electron microscopy (FE-SEM, Model S-4800, Hitachi Co., Ltd., Japan). Magnetic properties of the MCMs were measured at room temperature using a vibrating sample magnetometer (VSM, Model 7410, Lake Shore Co., Ltd., USA). Nitrogen adsorption and desorption performance were performed using a specific surface area analyzer (Model Coulter SA3100, Beckman Co., Ltd., USA). The surface areas were calculated using the Brunauer–Emmett–Teller (BET) equation. Surface zeta potential was measured by a zeta potential analyzer (ZS90, Malvern Instruments, UK).
The Reusability Method of MCMs
To assess the reusability of MCMs, 1 g/L MCMs was added in 25 mg/L sulfanilamide solution in which its concentration of pharmaceutical plant drainage was simulated. The adsorption capacity of MCMs was calculated when the adsorption reached equilibrium. The absorbed MCM could be separated and dispersed in distilled water and desorbed by adding 0.1 mol/L NaOH until the pH value reached 10.0, then ultrasounded at 500 W for 10 min, and this process was repeated three times [19, 20]. Then, MCMs were washed by distilled water repeatedly till the pH = 7. In all the experiments, the magnet was employed to separate MCMs from aqueous solution.
Results and Discussion
TEM of MCMs
As shown in Fig. 1a, the sizes of Fe3O4 nano/microspheres were around 200 nm and dispersed uniformly. After Fe3O4 nano/microspheres were reacted with glucose by hydrothermal method, the carbon was covered on the surface of Fe3O4 microspheres (Fig. 1b). At the same time, some carbon microspheres were formed which was in accordance with previous works of Cakan et al. .
FT-IR and XRD Spectrum of MCMs
The resulting Fe3O4 and MCMs had adsorption peak near 574 cm−1, which was the characteristic peak for Fe3O4. There was a wide absorption peak near 3462 cm−1 for Fe3O4 and MCMs, which suggested the resulting Fe3O4 and MCMs had –OH functional group. The peaks in 1701 and 1621 cm−1 were vibration absorption of carbonyl and alkene, which attributed to carbonization of glucose in hydrothermal method.
It is found that all the reflection peaks can be assigned to the diffraction from (2 2 0), (3 1 1), (4 0 0), (4 2 2), (5 1 1), and (4 4 0) crystal planes of cubic structure of Fe3O4 (JCPDS no. 19-0629), which indicated the formation of magnetite nanoparticles .
Surface Area and Porous Volume of MCMs
The parameters of MCMs obtained at different reaction conditions
S BET (m2/g)
Pore volume (cm3/g)
Pore size (nm)
Impregnation 1 h, 550
Impregnation 1 h, 600
As shown in Fig. 3a, the adsorption curve of MCMs without ZnCl2 impregnation and calcination belonged to the II-type adsorption isotherm, which usually presented non-porous material; the hysteresis loop could be assigned to type H2 according to the IUPAC nomenclature, which implied that the porous volume was formed by packing of grains . At the same time, the sample in Fig. 3a possessed low surface area (223 m2/g) and low porous volume (0.082 m2/g), although it had a large porous size (3.7 nm), which confirmed the porosity were the packing porosity but not the primary porosity.
The MCM samples in Fig. 3b–d were all calcined at high temperature and had similar adsorption isotherms. As shown in Fig. 3, all the isotherm curves increased rapidly at low relative pressure, which implied there were micropores in the MCM samples and facilitated to strong adsorption; while at high relative pressure, these curves exhibited a plateau, which demonstrated that no further adsorption took place, and these curves were the typical I-type adsorption isotherm. In the adsorption–desorption procedure, there appeared hysteresis loop at the high relative pressure. The phenomenon suggested the presence of micropores or mesopores and the hysteresis loop could be classified into type H4. This type hysteresis loop usually appears on activated carbon . The corresponding pore size distribution data calculated by the BJH method showed that the pore size mainly distributed below 3–5 nm, which just confirmed that large amounts of mesopores exist on the surface of the MCMs. Although all the three MCM samples had the similar adsorption isotherm as activated carbon, their surface areas and porous volumes were different, as listed in Table 1.
Compared with the MCM samples (c) and (d), MCM samples (b) had much lower surface area (356 m2/g) and porous volume (0.175 cm3/g), which were calcined at 550 °C for 1 h without ZnCl2 impregnation. Therefore, it can be concluded that ZnCl2 played a vital role in increasing the surface area and porous volume. As previously reported, ZnCl2 is used for activate agents in preparation process of activated carbon and can result in degradation of cellulosic material and dehydration, which can cause charm and aromatization of the carbon skeleton and creation of the pore structure . Furthermore, the MCM samples (c) and (d) were all impregnated 1 h, and the only one difference was their calcination temperature, which led to the surface area and porous volume being changed significantly. The higher the temperature, the greater the surface area and porous volume. So the MCM samples (d) were chosen for the following magnetic properties and adsorption research because of its highest surface area and porous volume.
Magnetic Properties of MCMs
As shown in Fig. 4, the saturation magnetization of the pure Fe3O4 nano/microspheres was 80.3 emu/g, which was smaller than 92.0 emu/g, the saturation magnetization of bulk Fe3O4 , while its saturation magnetization of MCMs was 42.3 emu/g, which was much less than that of pure Fe3O4 nano/microspheres and bulk Fe3O4. This sharp decrease indicated there was much carbon adhered to the surface of Fe3O4 nano/microspheres. However, the magnetic cores in MCMs possessed high saturation magnetization, the carbon which adhered to the surface of Fe3O4 nano/microspheres almost had no effects on their magnetic responsibility. Their remnant magnetization and coercivity were found to be zero, indicating Fe3O4 nano/microspheres and MCMs were superparamagnetic, which implied that the MCMs could be controlled and separated by using applied magnetic field.
The relevant parameters of the two models
Q m (or n)
K L = 3.264
Q m = 27.8551
K F = 3.0564
n = 2.099
As shown in Fig. 5 and Table 2, there was a linear relationship in the Langumir and Freundlich isotherm models and had no big difference in the two models. In the Langumir model, the theoretical maximum adsorption capacity of MCMs for sulfonamide was Q m = 27.8551 mg/g. In the Freundlich model, the values of the constants K F and 1/n were calculated to be 3.0564 L/g and 0.476, respectively. Since the value of 1/n is less than 1, it indicated a favorable adsorption. As far as the linear coefficient value (R 2) was concerned, compared with the Freundlich model, the linear coefficient value (R 2) of the Langmuir isotherm model was greater than the other one, which indicated that the equilibrium adsorption data fitted the Langmuir isotherm better.
The kinetic curves and the calculated parameters of the adsorption kinetic models
Y = − 0.147X + 2.622
Y = 0.039X + 0.085
K 1 = 0.147
K 2 = 0.0179
As shown in this Table 3, the correlation coefficient in the pseudo-second-order equation was more than that of the pseudo-first-order model and showed good linearity, which indicated that the adsorption of sulfonamide by MCMs was likely kinetically controlled as a second-order reaction rather than a first-order one, and the adsorption rate-limiting step may include chemisorption.
Effects of pH Values on MCMs’ Adsorption Capacity
MCMs’ adsorption capacity was influenced by the sulfanilamide speciation and the charges in the surface of MCMs. As shown in Fig. 6, the adsorption capacity of MCMs was reduced from 24.22 to 12.48 mg/g when the pH was increased from 4 to 12. The higher adsorption performance in acid solution than in alkaline solution may be related to the pKa of sulfonamide and zero point potential of MCMs. When the pH was in the range of 4.0~6.0 which was in the acidic condition, its zeta potential was 2.96 mV, the surface of MCMs was mainly positive charge, and the sulfanilamide existed mainly by natural molecular state (sulfonamide0) at the same time [28, 29]. Thus, sulfonamide could be easily absorbed onto MCMs, which indicated MCMs had a higher removal efficiency than those in alkaline condition; while in the alkaline condition, its zeta potential was − 4.01 mV, the positive charge on the surface of the MCMs was modified into negative charge, and the sulfanilamide speciation was varied into negative ones (sulfonamide−), which led to the electrostatic repulsion effect between sulfonamide species and MCMs because of their same kind of charges. Furthermore, sulfanilamide was easily dissolved in the alkaline solution , which made it having more tendency to dissolve in the solution rather than be absorbed to the MCMs. Therefore, the adsorption capacity was decreased significantly, which implied that MCMs can be desorbed effectively in alkaline solution, such as pH = 10.
Effects of Temperature and Ion Strength on MCMs’ Adsorption Capacity
Effects of temperature and ion strength on MCMs’ adsorption capacity
Adsorption capacity comparison of MCMs with other absorbents reported for sulfonamide
This comparison suggests that MCMs can serve as an alternative absorbate in removing sulfonamide. At the same adsorption conditions, the adsorption capacity of resulting MCMs and Fe3O4 nanoparticles was 24.22 and 10.83 mg/g, respectively, which means its adsorption capacity of MCMs mainly comes from carbon.
The Reusability of MCMs
As shown in Fig. 7, the adsorption removal efficiency was 94.28%, and its adsorption capacity for sulfonamide was calculated to be 23.6 mg/g. After being washed with diluted NaOH solution and reused, its adsorption efficiency was decreased with the recycling number increasing. The obtained adsorption removal efficiencies were 85.23, 81.17, 76.53, and 73.23% for the second-, third-, fourth-, and fifth-time adsorption, respectively, which were corresponding to 21.31, 20.29, 19.13, and 18.31 mg/g of adsorption capacity. Comparing Fig. 7b with Fig. 1b, morphology and microstructures of the MCMs after reused four times were not changed. Consequently, MCMs could be reused for sulfanilamide removal.
The MCMs possessing sensitive magnetic responsibility and high surface area were successfully synthesized by a facile hydrothermal method, and its specific surface area and pore volume reached up to 1228 m2/g and 0.445 m3/g, respectively. The adsorption of sulfanilamide by MCMs fitted well with the Langmuir isotherm model and followed pseudo-second-order kinetics. After being desorbed with NaOH solution, the adsorbent of MCMs could be recycled. The main findings of the present work will contribute to designing and synthesizing novel absorbents, and a better understanding of their adsorption physicochemical processes.
We acknowledge the financial support received from the National Natural Science Foundation of China (41473071), the High Level Talent Project of “Six Talents Summit” in Jiangsu Province (JNHB-008), the Jiangsu Environmental Protection Project (No. 2015070), the National-Local Joint Engineering Research Center for Biomedical Functional Materials, and the Priority Academic Program Development of Jiangsu Higher Education Institutions (PAPD, 164320H116) for this study.
FW and WJ designed the experiments. YC and JM performed the experiments. WD and JB participated in analyzing the data. WD, FHW, JM, and WJ wrote the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Kummerer K (2001) Drugs in the environment: emission of drugs, diagnostic aids and disinfectants into wastewater by hospitals in relation to other sources: a review. Chemosphere 45:957–969View ArticleGoogle Scholar
- Heberer T (2002) Occurrence, fate, and removal of pharmaceutical residues in the aquatic environment: a review. Toxicol Lett 131:5–17View ArticleGoogle Scholar
- Jones OAH, Voulvoulis N, Lester JN (2001) Human pharmaceuticals in the aquatic environment: a review. Environ Technol 22:1383–1394View ArticleGoogle Scholar
- Kim SC, Carlson K (2007) Temporal and spatial trends in the occurrence of human and veterinary antibiotics in aqueous and river sediment matrices. Environ Sci Technol 41:50–57View ArticleGoogle Scholar
- Stoob K, Singer HP, Mueller S (2007) Dissipation and transport of veterinary sulfonamide antibiotics after manure application to grassland in a small catchment. Environ Sci Technol 41:7349–7355View ArticleGoogle Scholar
- Li B, Zhang T (2010) Biodegradation and adsorption of antibiotics in the activated sludge process. Environ Sci Technol 44:3468–3473View ArticleGoogle Scholar
- Fang Y, Ni Y, Zhang G, Mao C, Huang X, Shen J (2012) Biocompatibility of CS–PPy nanocomposites and their application to glucose biosensor. Bioelectrochemistry 88:1–7View ArticleGoogle Scholar
- Smart SK, Cassady AI (2006) The biocompatibility of carbon nanotubes. Carbon 44:1034–1047View ArticleGoogle Scholar
- Zhu Q, Chen L, Zhu P, Luan J, Mao C, Huang X, Shen J (2013) Preparation of PNIPAM-gP (NIPAM-co-St) microspheres and their blood compatibility. Colloid Surf B 104:61–65View ArticleGoogle Scholar
- Gilani N, Daryan JT, Rashidi A, Omidkhah MR (2012) Separation of methane–nitrogen mixtures using synthesis vertically aligned carbon nanotube membranes. Appl Surf Sci 10:4819–4825View ArticleGoogle Scholar
- Serp P, Corrias M, Kalck P (2003) Carbon nanotubes and nanofibers in catalysis. Appl Catal A Gen 2:337–358View ArticleGoogle Scholar
- Ania CO, Cabal B, Pevida C, Arenillas A, Parra JB, Rubiera F, Pis JJ (2007) Effects of activated carbon properties on the adsorption of naphthalene from aqueous solutions. Appl Surf Sci 13:5741–5746View ArticleGoogle Scholar
- Wu S, Huang J, Ci Z, Zhang F, Sheng W, Zhu M (2016) One-step fabrication of magnetic carbon nanocomposite as adsorbent for removal of methylene blue. J Inorg Organomet Polym 26:632–639View ArticleGoogle Scholar
- Zhu Y, Zhang L, Schappacher FM (2008) Synthesis of magnetically separable porous carbon microspheres and their adsorption properties of phenol and nitrobenzene from aqueous solution. J Chem Phys 112:8623–8628Google Scholar
- Zhu M, Diao G (2011) Review on the progress in synthesis and application of magnetic carbon nanocomposites. Nano 3:2748–2767Google Scholar
- Zhu M, Diao G (2011) Synthesis of porous Fe3O4 nanospheres and its application for the catalytic degradation of xylenol orange. J Phys Chem C 115:18923–18934View ArticleGoogle Scholar
- Hu ZH, Srinivasan MP, Ni YM (2001) Novel activation process for preparing highly microporous and mesoporous activated carbons. Carbon 39:877–886View ArticleGoogle Scholar
- Saka C (2012) BET, TG-DTG, FT-IR, SEM, iodine number analysis and preparation of activate carbon from acorn shell by chemical activation with ZnCl2. J Anal Appl Pyrol 95:21–24View ArticleGoogle Scholar
- Hamdaoui O, Djeribi R, Naffrechoux E (2005) Desorption of metal ions from activated carbon in the presence of ultrasound. Ind Eng Chem Res 44:4737–4744View ArticleGoogle Scholar
- Li YH, Di ZC, Ding J (2005) Adsorption thermodynamic, kinetic and desorption studies of Pb2+ on carbon nanotubes. Water Res 39:605–609View ArticleGoogle Scholar
- Cakan RD, Baccile N, Antonietti M (2009) Carboxylate-rich carbonaceous materials via one-step hydrothermal carbonization of glucose in the presence of acrylic acid. Chem Mater 21:484–490View ArticleGoogle Scholar
- Gu J, Jiang W, Wang F, Chen M, Mao J, Xie T (2014) Facile removal of oils from water surfaces through highly hydrophobic and magnetic polymer nanocomposites. Appl Surf Sci 301:492–499View ArticleGoogle Scholar
- Sing KSW, Everett DH, Haul RAW (1982) Reporting physisorption data for gas/solid systems. Pure Appl Chem 11:2201–2218Google Scholar
- Sudaryanto Y, Hartono SB, Irawaty W (2006) High surface area activated carbon prepared from cassava peel by chemical activation. Bioresour Technol 97:734–739View ArticleGoogle Scholar
- Caturla F, Molina-Sabio M, Rodríguez-Reinoso F (1991) Preparation of activated carbon by chemical activation with ZnCl2. Carbon 29:999–1007View ArticleGoogle Scholar
- Bao J, Fu Y, Bao Z (2013) Thiol-functionalized magnetite/graphene oxide hybrid as a reusable adsorbent for Hg2+ removal. Nanoscale Res Lett 8:486View ArticleGoogle Scholar
- Wang FH, Jiang W, Fang Y, Cheng CW (2015) Preparation of Fe3O4 magnetic porous microspheres (MPMs) and their application in treating mercury-containing wastewater from the polyvinyl chloride industry by calcium carbide method. Chem Eng J 259:827–836View ArticleGoogle Scholar
- Ji L, Chen W, Zheng S, Xu Z, Zhu D (2009) Adsorption of sulfonamide antibiotics to multiwalled carbon nanotubes. Langmuir 25:11608–11613View ArticleGoogle Scholar
- Zhao YP, Gu XY, Gao SX, Geng JJ, Wang XR (2012) Adsorption of tetracycline (TC) onto montmorillonite: cations and humic acid effects. Geoderma 183:12–18View ArticleGoogle Scholar
- Kinnle KH, Sayward JI (1942) Solubilities of orthanilamide, metanilamide and sulfanilamide. J Am Chem Soc 64:2464–2468View ArticleGoogle Scholar
- Shi P, Ye N (2015) Investigation of the adsorption mechanism and preconcentration of sulfonamides using a porphyrin-functionalized Fe3O4-graphene oxide nanocomposite. Talanta 143:219–225View ArticleGoogle Scholar
- Korzh EA, Smolin SK, Klymenko NA (2016) Impact of characteristic of activated carbons on the efficiency of removal from water of pharmaceutical preparations of various chemical nature. J Water Chem Technol 38:83–88View ArticleGoogle Scholar
- Kochuk EV, Dmitrienko SG (2011) Sorption of sulfanilamides on highly cross-linked polystyrene. Russ J Phys Chem A 85:89–93View ArticleGoogle Scholar